A Carpet Cloak for Visible Light † ^ † ^ ‡ † † § Majid Gharghi, , Christopher Gladden, , Thomas Zentgraf, Yongmin Liu, Xiaobo Yin, Jason Valentine, † || and Xiang Zhang*, , † NSF Nanoscale Science and Engineering Center (NSEC), University of California, Berkeley 3112 Etcheverry Hall, UC Berkeley, California 94720, United States ‡ Department of Physics, University of Paderborn, Warburger Strasse 100, 33098 Paderborn, Germany § Department of Mechanical Engineering, Vanderbilt University, VU Station B 351592, Nashville, Tennessee 37235, United States Materials) Science Division, Lawrence Berkeley National Laboratory, 1 Cyclotron Road, Berkeley, California 94720, United States
ABSTRACT: We report an invisibility carpet cloak device, which is capable of making an object undetectable by visible light. The cloak is designed using quasi conformal mapping and is fabricated in a silicon nitride waveguide on a specially developed nanoporous silicon oxide substrate with a very low refractive index (n<1.25). The spatial index variation is realized by etching holes of various sizes in the nitride layer at deep subwavelength scale creating a local eﬀective medium index. The fabricated device demonstrates wideband invisibility throughout the visible spectrum with low loss. This silicon nitride on low index substrate can also be a general scheme for implementation of transformation optical devices at visible frequencies. KEYWORDS: Optical metamaterials, invisibility cloak, transformation optics, nanofabrication
nvisibility cloaks, a family of optical illusion devices that route broadband loss-less design and may be invariably extended in the Ielectromagnetic (EM) waves around an object so that the third dimension with some limitations,21 experimentally demon- existence of the object does not perturb light propagation, are still strated to operate for a range of viewing angles.19 The relatively in their infancy. Artiﬁcially structured materials with engineered modest material requirements dictated by QCM enabled the EM properties, known as metamaterials,1,2 have been used to implementation of the cloaking devices in the infrared20,21 using control the propagation of EM waves. Metamaterials have been a silicon waveguide. The index variation in these systems is applied to cloaking using the transformation optics design realized through a spatial modulation of the ﬁlling fraction of À methodology3 to control the propagation of optical4 8 and more dielectrics at subwavelength dimensions, providing a weighted À recently plasmonic9 11 waves. The invariance of Maxwell’s average index according to the eﬀective medium approximation. equations under coordinate transformation3 allows the space At shorter wavelengths however, devices reported so far suﬀer around an object to be reshaped such that the light can propagate from signiﬁcant scattering from surfaces within a unit cell as the in the desired manner. Such transformations usually require EM feature sizes become comparable to wavelength. More impor- properties with extreme values that are only achievable in tantly, the silicon device layer employed in the infrared becomes metallic metamaterials and have been experimentally demon- lossy due to absorption at visible frequencies. To realize cloaking strated for cloaking at microwave frequencies.12,13 Because of the at visible frequencies, the unit cell size must be reduced and a new ﬁ material system is required that provides both transparency and signi cant metallic loss at optical frequencies, the implementa- ﬃ tion of invisibility cloaks for visible light has been diﬃcult. su cient index contrast. We demonstrate here a visible light Recently another innovative strategy was developed based on carpet cloak device made of silicon nitride on a specially prepared exploiting uniaxial crystals.14,15 These devices have demonstrated nanoporous silicon oxide with very low index of <1.25. This cloaking in visible frequencies for a certain polarization of light unique substrate increases the available index modulation and enables the implementation of transformation optics for guided based on intrinsic anisotropy in the crystals. 16 visible light. As an alternative, conformal mapping, in which an inverse The optical transformation is designed so that a bump centered transformation of the electrical permittivity and magnetic perme- at the origin and deﬁned analytically as y = h cos2(πx/w) ability leads to a spatially variable refractive index proﬁle, can be 17 with a height h of 300 nm and a width w of 6 μm is compressed applied to cloaking. A two-dimensional (2D) quasi conformal in the y direction (inset of Figure 1a). QCM of the transformed mapping (QCM) technique can be employed to numerically space results in the relative index variation shown in Figure 1a. minimize the anisotropy in the index proﬁle which results from The smallest index values occur at the corners of the bump and the optical transformation. 2D QCM is the basis for the carpet 18 the maximum index appears around the top of the curved region. cloak, in which an object is hidden under a reﬂective layer (the carpet). To achieve cloaking, the raised protrusion (the bump) created in the reﬂective layer is mapped to a ﬂat plane and the Received: April 9, 2011 resulting 2D index proﬁle forms a carpet cloak device. In contrast Revised: May 15, 2011 to resonant optical structures,19,20 QCM carpet cloak provides a Published: May 27, 2011
r 2011 American Chemical Society 2825 dx.doi.org/10.1021/nl201189z | Nano Lett. 2011, 11, 2825–2828 Nano Letters LETTER
Figure 1. (a) Index variation for the optical transformation of a “bump” to a ﬂat plane, normalized to index 1; the eﬀective index of the cloak is found by multiplying the index shown by the desired background index; the inset schematically shows the transformation performed. (b) Requirements on the index variation and substrate index for implementing the cloaking transformation in the infrared (silicon waveguide on silicon oxide substrate) and the visible (silicon nitride waveguide on low index substrate). Solid line indicates the index of the unmodiﬁed material, while the shaded region below the solid line shows the range of index Δn that must be available. At visible frequencies, a new substrate material is needed as the index variation required for a silicon nitride waveguide goes below the index of the conventional silicon oxide substrate. The inset shows the feature size requirement for scattering free propagation of light in the metamaterial as a function of wavelength, which is used as a design criteria for the cloak.
Figure 2. (a) Cross sectional schematic of the cloak device implemented in a silicon nitride waveguide on a low index nanoporous silicon oxide substrate; the nitride layer and the nanoporous oxide layer are 300 nm and 5À10 μm thick, respectively. The hole pattern allows for index modulation by varying the solid ﬁlling fraction. The holes vary in size from 65 to 20 nm. The inset shows an SEM image of the low index nanoporous silicon oxide substrate. (b) AFM image of the hole pattern as transferred to the electron beam resist after development; the smallest holes appear shallow due to incomplete penetration of the AFM tip, but based on the uniform pattern transfer we conclude that they are completely through the resist. (c) SEM image of the device, consisting of roughly 3000 holes; the optical transformation device is surrounded by a triangular background index region not pictured.
Away from the bump, the index converges to the relative back- 130 nm pitch, thereby changing the ﬁlling fraction of air/SiN ground index of 1. The actual index variation Δn and the mixture. A waveguide thickness of 300 nm is chosen to achieve background index in the ﬁnal device depend on the materials single mode propagation while maintaining suﬃcient index used. Figure 1b shows the index modulation and the substrate contrast for strongly conﬁned modes at longer wavelengths. This index required to achieve cloaking, highlighting the requirements will result in the fundamental transverse electric mode index to implement the carpet cloak in the visible spectrum. It is varying from 1.83 to 1.74 for wavelengths of 400 nm to 700 nm. important to note that the silicon oxide substrate index fails to Thus the background index calculated for the transformation in provide enough contrast for waveguiding at visible frequencies. Figure 1a was projected to approximately 1.5. Figure 2a shows a To achieve the required index contrast, we consider silicon cross-sectional schematic of the device with the hole size pattern nitride (SiN) waveguide on a specially developed low index generated to achieve the required index modulation. As expected, substrate made from nanoporous silicon oxide. The inset in the largest holes are located at the corners of the bump and the Figure 1b shows the approximate unit cell size requirement for smallest holes appear right above the peak of the bump. the scattering-free operation of the eﬀective medium. In order for Additionally, an area of constant hole size surrounding the cloak the device to operate throughout the visible spectrum, feature device is required to provide a uniform background index. sizes should be on the order of 65 nm half pitch. The device fabrication process begins with the preparation of In visible frequencies, our SiN has a bulk refractive index of the low index substrate. A crystalline silicon wafer is electro- approximately 1.9 and the nanoporous silicon oxide substrate has chemically etched in an acid/organic (1:1 hydroﬂuoric acid/ an exceptionally low refractive index of <1.25 and both are ethanol) solution to produce a porous network that penetrates transparent. To modulate the index of the SiN waveguide, several micrometers into the top surface. The porosity of this variable-sized holes were drilled in a 2D hexagonal lattice with network is increased by oxidizing several atomic layers of silicon
2826 dx.doi.org/10.1021/nl201189z |Nano Lett. 2011, 11, 2825–2828 Nano Letters LETTER on the internal surfaces at 300 C and subsequently removing this oxide layer by selective etching. By repeating the oxidation and etching several times, the solid silicon is slowly consumed, leaving solid ﬁlling fractions as low as 15%. Once the desired porosity is reached, the entire silicon network is converted to a porous silicon oxide medium by oxidizing at high temperature (800 C). Because of expansion during oxidation, the resulting medium turns into an approximately 65% porous glass, where the pores range in size from 2 to 20 nm (shown in the inset of Figure 2a). The resulting substrate has a refractive index below 1.25, as conﬁrmed by optical interference measurement in the near-infrared, and has a smooth surface with roughness less than 3 nm rms. A 300 nm SiN slab waveguide is deposited on the low index substrate using plasma-enhanced chemical vapor deposi- tion (PECVD). To fabricate the hole pattern introduced in Figure 2a, we use a two step pattern transfer process. The waveguide is ﬁrst covered with a 100 nm thick PECVD silicon oxide to act as a hard mask Figure 3. (a) Optical characterization setup; the half-wave plate rotates for etching. ZEP520A electron beam resist is then spun on the the polarization of the laser output as desired; the out-coupled light oxide layer with a thickness of 120 nm, and the generated hole polarization is rotated 90 due to the reﬂection from the mirror in the pattern is written on the resist by electron beam lithography. sample, and the output polarizer is used to partially ﬁlter out the Figure 2b shows an atomic force microscope (AFM) image of the scattered input beam. Inset shows an SEM image of the gratings; the developed resist with the hole sizes varying from 65 to 20 nm. area behind the cloak has been etched by FIB and a silver layer has The resist is used as a mask to transfer the pattern to the 100 nm covered the back of the bump. (b) Dark-ﬁeld image of the cloak device oxide layer by reactive ion etching (RIE). The resist is then ashed with the input and output gratings. The input grating and beam path are and the pattern is transferred to the nitride waveguide using a highlighted by the green circle and the green arrows respectively. (c) Dark-ﬁeld image of the in coupling laser and the out-coupled light. The selective RIE process, followed by removal of the oxide mask. A low ﬁ pressure (18 mTorr) RIE etch was developed for directional yellow dashed triangle de nes the region containing the cloak. The red dashed rectangle indicates the out-coupling grating, which is the region pattern transfer to the nitride, for which close to 90 sidewall was of interest for the results presented in Figure 4. conﬁrmed by cross sectional imaging. Figure 2c shows an overall scanning electron microscope (SEM) image of the fabricated structure excluding a triangular region deﬁning the background a simple mirror without a bump. To characterize the perfor- index. To achieve a reﬂective bottom plane for the device, the area mance of the cloaking transformation, the reﬂection of the ﬂat under the bump is opened to the edge of the die using focused ion mirror, the noncloaked bump, and the cloak device are shown in beam (FIB) milling. The structure is then mounted at 90 angle Figure 4 for three diﬀerent excitation wavelengths of 480, 520, and a directional deposition is performed using electron beam and 700 nm. The 700 nm beam is the direct output from the Ti- evaporation to cover the bottom of the bump with silver. Sapphire laser, whereas the other two are the outputs of the The optical characterization setup is depicted in Figure 3a. For second harmonic generation in the OPO, and thus the beam exciting optical modes in the waveguide, we use a pulsed proﬁles are slightly diﬀerent at each wavelength. The ﬁgure also femtosecond (fs) Ti-Sapphire laser (Spectra Physics MaiTai) shows the simulated propagation pattern of a 600 nm wavelength along with an optical parametric oscillator (Spectra Physics Gaussian beam impinging on the system in the absence (cloak Inspire OPO) as the source. To couple light into and out of oﬀ) and the presence (cloak on) of the transformation. As seen in the waveguide, two gratings are made parallel to the sides of the the experimental results shown in Figure 4c, the reﬂection from triangle (inset Figure 3a). This design minimizes scattering from the noncloaked bump shows a clear perturbation in the wave- corners and keeps the propagation normal to all abrupt inter- front when compared to the reﬂection from the ﬂat mirror. The faces. The gratings consist of three periods to allow relatively cloak device on the other hand, reconstructs the wavefront broadband coupling across the visible spectrum. The laser beam producing a beam proﬁle identical to the original Gaussian beam was focused on the input grating through a 50Â dark-ﬁeld reﬂected from the ﬂat mirror. This conﬁrms that the designed objective, and the light collected from the output grating transformation eﬀectively cloaks the uneven surface throughout was imaged using a charge-coupled device (CCD) camera the entire visible spectrum, successfully rendering any object (Figure 3c). Since the input beam scatters at the in-coupling behind it invisible in the far ﬁeld. To further test the device, the grating, a polarizing ﬁlter aligned to the output grating was placed beam was also scanned along the length of the input grating to in front of the CCD to reduce the intensity of the image of the ensure the beam proﬁle on the output grating is not perturbed. input beam while not aﬀecting the output beam. The coupling The proposed cloak structure is inherently wideband and low- and the propagation of the beam in the slab waveguide were loss. However, the fabricated device has some limitations. The checked using two parallel gratings (transmission mode) in all nitride material becomes lossy due to absorption as we approach the conﬁgurations. In an actual experiment, besides the nonperfect ultraviolet region. Also, the waveguide conﬁnement at longer coupling at the gratings, there is a small additional loss due to the wavelength reduces the mode index, creating a waveguide cutoﬀ reﬂection at each of the triangle sides. However all such losses are in the infrared. Although the waveguide test structure and coupling extrinsic to the transformation device. gratings were designed for demonstration of the cloaking eﬀect Two control samples were also fabricated beside the cloak using light with transverse electric polarization, in principle the sample, a bump structure without any transformation pattern and QCM transformation operates for both polarizations.18,19,20
2827 dx.doi.org/10.1021/nl201189z |Nano Lett. 2011, 11, 2825–2828 Nano Letters LETTER
’ REFERENCES (1) Pendry, J. B.; Holden, A. J.; Robbins, D. J.; Stewart, W. J. Magnetism from Conductors and Enhanced Non-Linear Phenomena. IEEE Trans. Microwave Theory Tech. 1999, 47, 2075–2084. (2) Smith, D. R.; Padilla, W. J.; Vier, D. C.; Nemat-Nasser, S. C.; Schultz, S. Composite Medium with Simultaneously Negative Perme- ability and Permittivity. Phys. Rev. Lett. 2000, 84, 4184–4187. (3) Pendry, J. B.; Schurig, D.; Smith, D. R. Controlling Electro- magnetic Fields. Science 2006, 312, 1780–1782. (4) Cai, W.; Chettiar, U. K.; Kildishev, A. V.; Shalaev, V. M. Optical Cloaking with Metatmaterials. Nat. Photonics 2007, 1, 224–227. (5) Rahm, M.; Cummer, S. A.; Shurig, D.; Pendry, J. B.; Smith, D. R. Optical Design of Reﬂectionless Complex Media by Finite Embedded Coordinate Transformations. Phys. Rev. Lett. 2008, 100, 063903. (6) Jiang, W. X.; Cui, T. J.; Yang, X. M.; Cheng, Q.; Liu, R.; Smith, D. R. Invisibility Cloak without Singularity. App. Phys. Lett. 2008, 93, 194102. (7) Kildishev, A. V.; Shalaev, V. M. Engineering Space for Light via Transformation Optics. Opt. Lett. 2008, 33,43–45. (8) Chen, H.; Ng, J.; Lee, C. W. J.; Lai, Y.; Chan, C. T. General Figure 4. Simulated propagation of a Gaussian beam when reﬂected Transformation for Reduced Invisibility Cloak. Phys. Rev. B 2009, from a bumped carpet (a) without and (b) with a cloaking device on top 80, 085112. of the carpet. The input beam indicated by the black arrow has a (9) Huidobro, P. A.; Nesterov, M. L.; Martín-Moreno, L.; García- wavelength of 600 nm. The perturbation caused by the bump is masked Vidal, F. J. Transformation Optics for Plasmonics. Nano Lett. 2010, by the cloak device and the reﬂected beam is reconstructed as if the 19, 1985–1990. bump did not exist. (c) Experimental results: normalized intensity CCD (10) Liu, Y.; Zentgraf, T.; Bartal, G.; Zhang, X. Transformational images of the out-coupled light (shown in false color) from the Plasmon Optics. Nano Lett. 2010, 10, 1991–1997. waveguide after reﬂection from a ﬂat mirror, bump without a cloak, (11) Aubry, A.; Lei, D. Y.; Fernandez-Domínguez, A. I.; Sonnefraud, and cloaked bump at three diﬀerent wavelengths. The bump clearly Y.; Maier, S. A.; Pendry, J. B. Plasmonic light-harvesting devices over the distorts the wavefront, creating a lobed pattern. The cloak successfully whole visible spectrum. Nano Lett. 2010, 10, 2574–2579. reconstructs the wavefront so that the output is unperturbed. (12) Schurig, D.; Mock, J. J.; Justice, B. J.; Cummer, S. A.; Pendry, J. B.; Starr, A. F.; Smith, D. R. Metamaterial Electromagnetic Cloak at Microwave Frequencies. Science 2006, 314, 977–980. In conclusion, we have demonstrated a full visible spectrum (13) Edwards, B.; Alu, A.; Silveirinha, M. G.; Engheta, N. Experi- transformation optical device that is capable of cloaking any object ﬁ ﬂ mental Veri cation of Plasmonic Cloaking at Microwave Frequencies underneath a re ective carpet layer. In contrast to the previous with Metamaterials. Phys. Rev. Lett. 2009, 103, 153901. demonstrations that were limited to infrared light, this work makes (14) Chen, X.; Luo, Y.; Zhang, J.; Jiang, K.; Pendry, J. B.; Zhang, S. actual invisibility for the light seen by the human eye possible. In Macroscopic Invisibility Cloaking of Visible Light. Nat. Comm. 2011, 2, 176. addition to successful demonstration of cloaking, the fabrication (15) Zhang, B.; Luo, Y.; Liu, X.; Barbastathis, G. Macroscopic scheme employed here is a signiﬁcant step toward general imple- Invisibility Cloak for Visible Light. Phys. Rev. Lett. 2011, 106, 033901. mentation of optical transformation structures in the visible range. (16) Leonhardt, U. Optical Conformal Mapping. Science 2006, 312, 1777–1780. Theconsiderableindexcontrastbetweenthewaveguideandthe New J. substrate enables realization of large index variations in the meta- (17) Leonhardt, U. Notes on Conformal Invisibility Devices. Phys. 2006, 8, 118. material device. In addition, the nitride waveguide on the low index (18) Li, J.; Pendry, J. B. Hiding under the carpet: A new strategy for substrate provides a platform for on-chip photonic devices in the cloaking. Phys. Rev. Lett. 2008, 101, 203901. visible range, which have been traditionally achievable in silicon (19) Alu, A.; Engheta, N. Multifrequency Optical Invisibility Cloak waveguide on oxide for the infrared. with Layered Plasmonic Shells. Phys. Rev. Lett. 2008, 100, 113901. (20) Smolyaninov, I. I.; Smolyaninova, V. N.; Kildishev, A. V.; ’ AUTHOR INFORMATION Shalaev, V. M. Anisotropic Metamaterials Emulated by Tapered Wave- guides: Application to Optical Cloaking. Phys. Rev. Lett. 2009, Corresponding Author 102, 213901. *E-mail: [email protected] (21) Landy, N. I.; Kundtz, N.; Smith, D. R. Designing Three- Dimensional Transformation Optical Media Using Quasiconformal Author Contributions Phys. Rev. Lett. 105 ^ Coordinate Transformations. 2010, , 193902. These authors contributed equally to this work. (22) Ergin, T.; Stenger, N.; Brenner, P.; Pendry, J. B.; Wegener, M. Three-dimensional invisibility cloak at optical wavelengths. Science 2010, 328, 337–339. ’ (23) Valentine, J.; Li, J.; Zentgraf, T.; Bartal, G.; Zhang, X. An optical ACKNOWLEDGMENT cloak made of dielectrics. Nat. Mater. 2009, 8, 568–571. The authors acknowledge funding support from the U.S. (24) Gabrielli, L. H.; Cardenas, J.; Poitras, C. B.; Lipson, M. Silicon ﬃ nanostructure cloak operating at optical frequencies. Nat. Photonics Army Research O ce (MURI programme W911NF-09-1- 3 – 0539). M.G. acknowledges fellowship from Natural Sciences 2009, , 461 463. and Engineering Research Council of Canada (NSERC). C.G. acknowledges support from NSF Graduate Research Fellowship Program (NSF GRFP). Devices fabricated in the UC Berkeley Marvell Nanofabrication Laboratory.
2828 dx.doi.org/10.1021/nl201189z |Nano Lett. 2011, 11, 2825–2828